# Inhomogeneous deformation in metallic glasses

←

**Page content transcription**

If your browser does not render page correctly, please read the page content below

Journal of the Mechanics and Physics of Solids 50 (2002) 1011 – 1027 www.elsevier.com/locate/jmps Inhomogeneous deformation in metallic glasses R. Huanga; b;∗ , Z. Suob; c , J.H. Prevosta; b , W.D. Nixd a Department of Civil and Environmental Engineering, Princeton University, Princeton, NJ 08544, USA b Princeton Materials Institute, Princeton University, Princeton, NJ 08544, USA c Department of Mechanical and Aerospace Engineering, Princeton University, Princeton, NJ 08544, USA d Department of Materials Science and Engineering, Stanford University, Stanford, CA 94305, USA Received 25 May 2001; accepted 29 August 2001 Abstract The present study provides a theoretical framework for the inhomogeneous deformation in metallic glasses. The free volume concentration is adopted as the order parameter, which is a function of position and time. The three processes that can change the local free volume concen- tration are di4usion, annihilation, and stress-driven creation. The rate functions for free volume generation and plastic 5ow depend on the underlying microscopic model, but the framework is generally valid for di4erent models. A simple shear problem is solved as an example. A linear stability analysis is performed on the basis of the homogeneous solution. An inhomogeneous solution is obtained with a 6nite amplitude disturbance to the initial free volume distribution. Numerical simulation shows the development of the inhomogeneous deformation and strain localization. ? 2002 Elsevier Science Ltd. All rights reserved. Keywords: Metallic glasses; Free volume; Inhomogeneous deformation; Localization 1. Introduction Metallic glasses, also known as amorphous metals, di4er from ordinary metals in that their atoms do not assemble on a crystalline lattice. Since the 6rst amorphous metal was formed from the liquid state of an Au–Si alloy by the fast quenching technique (Klement et al., 1960), a great number of amorphous metals have been produced during the last three decades. Prior to the development of bulk metallic glasses, very high cooling rates (¿105 K=s) were required to prevent crystallization and studies of metallic glasses were con6ned to very thin ribbons or wires (Pampillo, 1975). The ∗ Correspondingauthor. Department of Civil and Environmental Engineering, Princeton University, Prince- ton, NJ 08544, USA. Tel.: +1-609-258-1619; fax: +1-609-258-1270. E-mail address: ruihuang@princeton.edu (R. Huang). 0022-5096/02/$ - see front matter ? 2002 Elsevier Science Ltd. All rights reserved. PII: S 0 0 2 2 - 5 0 9 6 ( 0 1 ) 0 0 1 1 5 - 6

1012 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 recent development of bulk metallic glasses (Johnson, 1999) has allowed mechanical testing under a much wider range of loading conditions and has renewed interest in this class of material. While many properties of bulk metallic glasses are still under active investigation, it has been con6rmed that metallic glasses have a unique combination of various properties and are suitable for many applications, ranging from sporting equipment (Onugi et al., 1999) to MEMS (Maekawa et al., 2000). Mechanical properties of metallic glasses have been studied for many years. Based on 5ow data for Pd-based metallic glasses from creep tests, uniaxial compression tests, and tensile tests, Spaepen (1977) has established an empirical deformation map. In the range in which the material can be considered a solid, two basic modes of deformation can be distinguished: homogeneous 5ow and inhomogeneous 5ow. Homogeneous 5ow occurs at low stresses and high temperatures as in creep tests (Chen and Goldstein, 1972). Under uniaxial tension, a specimen thins down uniformly during deformation. Inhomogeneous 5ow occurs at high stresses and low temperatures, where the strain localizes in a few very thin shear bands. In uniaxial tensile tests, metallic glasses exhibit very high yield strength compared to crystalline metals, but fracture occurs along a single band with little global plasticity (Leamy √ et al., 1972). Meanwhile, fracture toughness values ranging from 16 to 55 MPa m have been measured using compact tension and single edge notched bend geometries (Conner et al., 1997; Gilbert et al., 1997; Lowhaphandu and Lewandowski, 1998). Even higher values of fracture toughness of a Zr–Ti–Ni–Cu–Be bulk metallic glass have been measured by using a single edge notched tension geometry (Flores and Dauskardt, 1999). The high fracture toughness of metallic glasses is associated with signi6cant plastic deformation and blunting formed by multiple shear bands and branched cracks. Multiple shear bands have also been observed in specimens loaded under other constrained geometries, such as uniaxial compression and bending (Pampillo, 1975; Hufnagel et al., 2000; Wright et al., 2001). By bonding a layer of metallic glass between two ductile metal layers, Leng and Courtney (1991) observed a high density of shear bands “trapped” between the ductile layers under tensile loading (tensile axis parallel to the layers). Recent study of a new class of ductile metal reinforced metallic glass matrix composites shows that organized shear band patterns develop throughout the sample under bending, compression, and tensile tests (Hays et al., 2000). Some theoretical models have been put forth to explain various features of the inhomogeneous deformation in metallic glasses. Argon (1979) has shown that 5ow can localize in a band in which the strain rate has been perturbed, when the threshold stress for driving the local shear transformations is altered through creation of free volume. Steif et al. (1982) assumed an initial band of slightly weaker material in their analysis of strain localization and shear band. However, the origin of such a band was not considered in detail. More recently, Vaks (1991) proposed a possible mecha- nism for the formation of shear bands in amorphous alloys at the stage preceding the macroscopic 5ow. To enable theoretical analysis for both the initial shear band formation and the post shear banding deformation, we provide a general framework within the context of continuum mechanics in the present study. In addition to the deviatoric plastic 5ow, we introduce an inelastic dilatational strain associated with the excess free volume as

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1013 another internal variable. Three processes compete to change the local free volume concentration and they are di4usion, annihilation, and stress-driven creation. As an example, a simple shear problem is studied in detail. Both homogeneous and inhomo- geneous solutions are obtained. A linear stability analysis is performed on the basis of the homogeneous solution. Numerical simulations of the inhomogeneous solution show the development of localized shear deformation. The plan of the paper is as follows. Section 2 describes the general formulation of the framework. In Sections 3 and 4, explicit formulae for the plastic 5ow and free volume generation are introduced based on a speci6c microscopic model. In Section 5, we consider the simple shear problem and discuss the homogeneous solution, linear stability analysis, and the inhomogeneous solution, respectively, in three subsections. Finally, some concluding remarks are given in Section 6. 2. General formulation In the absence of body forces, momentum balance requires that 92 ui ij; j = ; (1) 9t 2 where the summation convention is used for i; j = 1; 2; 3, and (); j denotes di4erentiation with respect to the jth spatial coordinate. ij are the components of the Cauchy stress tensor, ui are the components of displacement, and is the mass density. Con6ning to the small deformation assumptions, the strain relates to the displacement gradients by ij = 12 (ui; j + uj; i ): (2) However, because the strain can be extremely large inside shear bands during inho- mogeneous deformation of metallic glasses, a more precise formulation should allow large strain. Nevertheless, Eq. (2) is used in this preliminary work. In the present model of metallic glasses, the total strain consists of three parts: the elastic strain ije , the deviatoric plastic strain ijp , and the inelastic dilatational strain associated with excess free volume, i.e., e p ij = ij + ij + 13 ( − 0 ) ij ; (3) where is the local concentration of free volume (to be de6ned shortly) and 0 is the free volume concentration at the reference state with zero strain. We assume the metallic glasses to be isotropic and specify the constitutive laws using the invariants of the stress tensor, such as the mean stress and the Mises e4ective shear stress. Dividing the stress tensor into the mean stress m = 13 (11 + 22 + 33 ) (4) and the deviatoric stress tensor sij = ij − m ij : (5)

1014 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 The Mises e4ective shear stress is e = 12 sij sij : (6) Next, we specify the constitutive laws for the elastic strain, the deviatoric plastic strain, and the inelastic dilatational strain in turn. The elastic strain relates to the stress by Hooke’s law. For isotropic materials, we have e e ij = 2 ij + ij ; (7) 1 − 2 kk where is the shear modulus and is Poisson’s ratio. The 5ow of the deviatoric plastic strain, ijp , is taken to be in the same direction as the deviatoric stress tensor sij , with the 5ow rate depending on the concentration of free volume , the e4ective shear stress e , and the mean stress m , namely, 9 ijp sij = f( ; e ; m ) : (8) 9t 2e The function f can be 6t to pure shear or uniaxial tensile tests. The inelastic dilatational strain is associated with the change of the local excess free volume. The excess free volume in metallic glasses is de6ned as follows. Let V be the volume of a sample and Vd be the volume of the same sample with a dense random packaging of atoms. The excess free volume, Vf , is the di4erence between the two volumes, i.e., Vf = V − Vd . De6ne the concentration of free volume as Vf = : (9) Vd In this paper, we take as the order parameter that describes the state of amorphous metals. To be speci6c, the free volume concentration is a continuum 6eld, which can be non-uniform and can evolve with time. There are three processes that can change the local free volume concentration: dif- fusion, annihilation, and generation. The di4usion of free volume is analogous to the di4usion of vacancies in crystalline materials. The free volume is redistributed by dif- fusion until it is spatially uniform. In crystalline materials, vacancies can annihilate at certain locations, such as grain boundaries and dislocations, where the structural requirement of crystalline translational symmetry is relaxed. In metallic glasses, this requirement does not exist and free volume can annihilate at any position simply by the atomic rearrangement. The annihilation of free volume decreases the total free volume and the metallic glasses become denser after annihilation. The generation of free volume is induced by stresses. Extra free volume can be created by a shear stress squeezing an atom into a hole smaller than itself (Spaepen, 1977). The combined rate of annihilation and generation of free volume, g, is taken to be a function of the local concentration of free volume , the e4ective shear stress e , and the mean stress m . Therefore, the change of free volume concentration is governed by a di4usion–production equation: 9 = D ; ii + g( ; e ; m ); (10) 9t

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1015 where the di4usivity D is a function of temperature, but is taken to be independent of the free volume concentration and the stresses. Eqs. (1) – (10) provide a general framework for inhomogeneous deformation in metal- lic glasses. The speci6c functions for the plastic 5ow, f( ; e ; m ), and the production rate of free volume, g( ; e ; m ), are discussed in the following two sections. Note that the functions are based on a speci6c microscopic model. As theories and exper- iments are re6ned, more appropriate functions may emerge. We will proceed within the general framework using the existing functions and leave detailed modi6cations to subsequent work. 3. Flow equation Based on the free volume theory Cohen and Turnbull (1959); Turnbull and Cohen, 1961, 1970; Spaepen (1977) derived a 5ow equation for metallic glasses under a shear stress : 9p v∗ OG m = 20 exp − − sinh ; (11) 9t vf kB T 2kB T where p is the plastic shear strain, vf the average free volume per atom, v∗ a critical volume (the e4ective hard-sphere volume of an atom, for example), a geometrical factor of order unity, 0 the frequency of atomic vibration, OG m the activation energy, the atomic volume, kB the Boltzmann’s constant, and T the absolute temperature. According to Eq. (11), the plastic strain rate increases as the applied shear stress increases. At a low stress, sinh 2k BT ≈ 2k BT , and Eq. (11) recovers the linear Newto- nian viscous behavior. Furthermore, the 5ow rate depends on the average free volume per atom. At a constant stress, the strain rate is higher when the average free vol- ume is larger. Changing the free volume can radically change the 5ow rate. Steif et al. (1982) showed that the softening induced by increasing the free volume permits localized deformation. For multiaxial stress states, we replace the shear stress in Eq. (11) with the Mises e4ective shear stress e . The concentration of free volume de6ned in Eq. (9) can be approximately taken as = vf =v∗ . Thus, from Eq. (11), we obtain a formula for the function f in the general 5ow Eq. (8) as below e f( ; e ) = 2R exp − sinh ; (12) 2kB T m where R = 0 exp − OG kB T and 1=R de6nes a time. Using the typical values of 0 ( ∼ 1013 s−1 ); OG m ( ∼ 10−19 J), and kB T ( ∼ 5 × 10−21 J, corresponding to T ∼ 400 K), we have R ∼ 2 × 104 s−1 . Note that the 5ow rate function in Eq. (12) is independent of the mean stress, m . Although the earlier work conducted on thin ribbons of amorphous Pd–Cu–Si reported a slight pressure dependence of the 5ow=fracture behavior, it was noted that there may have been problems with alignment and gripping which facilitated deformation

1016 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 and fracture at the grip ends (Davis and Kavesh, 1975). The recent study on the 5ow and fracture behavior of a Zr–Ti–Ni–Cu–Be bulk metallic glass showed that the 5ow stress and fracture strain are essentially independent of superimposed hydrostatic pressure over the range from 50 to 575 MPa (Lowhaphandu et al., 1999). However, the pressure is low compared to the yield stress of metallic glasses (1–2 GPa) and one might reasonably expect that the e4ect could only become important at higher pressures. Flores and Dauskardt (2001) showed in their experiments a critical tensile mean stress of 0:95 GPa and proposed a strain localization model with the e4ect of mean stress. While the mean stress e4ect on the 5ow behavior of metallic glasses is still under investigation, in the present study we include the e4ect in the 5ow equation for the general scheme (Eq. (8)), but set it to be zero in the example problem. 4. Free volume creation and annihilation The concentration of free volume plays the role as an order parameter in the present framework. An as-prepared metallic glass is thermodynamically unstable and has a non-equilibrium amount of free volume. The free volume is continuously being anni- hilated by structural relaxation toward the metastable equilibrium con6guration (Taub and Spaepen, 1980). Meanwhile, applying stresses can create free volume. In the model by Spaepen (1977), free volume is created by an applied shear stress and annihilated by a series of atomic jumps, and the net rate of the change of free volume is 9vf OG m v∗ 2kB T 1 = v∗ 0 exp − − cosh −1 − ; (13) 9t kB T vf Svf 2kB T nD where nD is the number of atomic jumps needed to annihilate a free volume equal to v∗ , and S = 32 1− 1+ . From Eq. (13), we obtain a formula for the function g in Eq. (10), again by taking = vf =v∗ and replacing with e , namely e 1 g( ; e ) = R exp − cosh −1 − ; (14) P 2kB T nD where 2 1 + v∗ = ; P = : (15) 31− 2kB T Notice that the e4ect of mean stress on the creation and annihilation of free volume has not been taken into account in Eq. (14). Equations modeling the e4ect of mean stress on free volume have been proposed by other studies (Steif, 1983; Flores and Dauskardt, 2001). Here, we include the e4ect in the general scheme (Eq. (10)), but neglect it in the following analysis. Fig. 1 schematically shows the rate function, Eq. (14), versus the free volume con- centration for constant e4ective shear stresses. When e = 0, there is no stress-driven creation of free volume and the concentration of free volume decreases as the result

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1017 Fig. 1. The combined rate function of annihilation and stress-driven creation of free volume from Spaepen’s microscopic model. of free volume annihilation. The rate is very small as the free volume concentration approaches zero, but the process does not stop until the free volume concentration is zero. However, since certain amount of free volume should exist in the metastable equilibrium con6guration to allow plastic 5ow, a better formula would have a non-zero equilibrium value of the free volume concentration. When e = 0, there exists a steady state, at which the stress-driven creation and the annihilation are balanced. The steady state value of the free volume concentration, E , increases as the e4ective shear stress increases. A comparison of the production rate in Eq. (14) with the di4usion term in the right-hand side of Eq. (10) de6nes a length: D l= : (16) R Thus, the di4usivity D takes the form OG m 2 D = 0 exp − l : (17) kB T Eq. (17) has the same form as the di4usivity for vacancies in crystalline materials, where the length scale is comparable to the diameter of atoms. Assuming the similar mechanism for the di4usion of free volume, we estimate l ∼ 0:1 nm. However, the mechanisms of free volume di4usion in metallic glasses are not well understood; in particular, it is not clear that the free volume di4uses by a vacancy-like mechanism. 5. Example: simple shear problem Consider a layer of width 2h (hl) in the x direction, as shown in Fig. 2. The dimensions of the layer in the y and z directions are much larger than h and are

1018 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 y h h τ x τ Fig. 2. Geometric con6guration of a simple shear problem. assumed to be in6nity. The layer is loaded with a constant average shear strain rate. The strain rate is assumed to be low, falling in the quasi-static range, such that we can neglect the inertial term in the momentum equation, Eq. (1). Under the quasi-static assumption, the force equilibrium requires that the shear stress be spatially uniform but time-dependent, i.e., = (t). As the shear stress creates more free volume, the sample dilates. When the dilation is non-uniform across the layer, geometric constraint will induce normal stresses in the y and z directions. The stresses are assumed equal in both directions, i.e., yy = zz = (x; t), and the total stress after integrating across the layer is zero h (x; t) d x = 0: (18) −h In the x direction, the material dilates freely with no constraint and the normal stress is zero. Under such a stress state, the e4ective shear stress is e = 2 + 13 2 : (19) The total shear strain, , consists of the elastic strain, e , and the plastic strain, p . The elastic shear strain relates to the shear stress by Hooke’s law, and the plastic strain 5ows according to Eq. (8). Thus, the total shear strain rate is 9 1 d = + f( ; e ) : (20) 9t dt e

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1019 The average shear strain rate is h 1 9 r= d x: (21) 2h −h 9t Integration of both the sides of Eq. (20) with respect to x from −h to h leads to h d 1 = r − f( ; e ) d x : (22) dt 2h −h e We assume that, by the geometric constraint, the normal strains are equal in the y and z directions and they are spatially uniform, i.e., yy = zz = (t). The normal strain consists of the elastic strain, the plastic strain, and the dilatational strain associated with free volume. The total normal strain rate is d 1 − 2 9 19 = + f( ; e ) + : (23) dt 2 9t 6e 3 9t By integrating both the sides of Eq. (23) with respect to x from −h to h and applying Eq. (18) for the 6rst term at the right-hand side, we obtain h d 1 19 = f( ; e ) + d x: (24) dt 2h −h 6e 3 9t Assuming that the concentration of free volume is uniform along the y and z direc- tions but varies along the x direction, Eq. (10) becomes 9 92 = D 2 + g( ; e ): (25) 9t 9x Eqs. (22) – (25) are coupled together and have to be solved simultaneously for the shear stress, the normal strain, the normal stress, and the free volume concentration. The shear strain can be computed from Eq. (20) after solving the coupled equations. 5.1. Homogeneous deformation If the initial distribution of the free volume is uniform across the layer, there exists a set of homogeneous solutions to Eqs. (22) – (25) and the deformation is homogeneous, i.e., h = rt; (26a) h = 0; (26b) dh = [r − f( h ; h )]; (26c) dt d h 1 = 3 g( h ; h ); (26d) dt d h = g( h ; h ): (26e) dt

1020 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 The shear strain in the above homogeneous solution is uniformly distributed, increas- ing linearly with time at the prescribed constant strain rate. Since the deformation is homogeneous, the normal stress due to the geometric constrain is zero and the normal strain is purely dilatational. The variations of the shear stress and the free volume con- centration with time are obtained by numerically integrating Eqs. (26c) and (26e) for the given strain rate, r. The solution is similar to that obtained by Steif et al. (1982) except for the normal strain in Eq. (26d). Fig. 3a shows the stress–strain curve of the homogeneous deformation and Fig. 3b shows the concentration of free volume versus the shear strain for normalized strain rate r=R = 10−6 . The initial concentration of free volume is taken to be 0.008 and the initial stress is zero. The material parameters used in the calculations are: P = 120; = 0:15; = 1; nD = 3. The shear stress drops after an initial elastic response and the free volume concentration increases concurrently, indicating a homogeneous softening of the material. The homogeneous deformation eventually reaches a steady state, at which both the free volume concentration and the shear stress are constant and the metallic glass 5ows like a liquid. The steady state values of the shear stress and free volume concentration correspond to the steady state point in Fig. 1 and depend on the prescribed strain rate. 5.2. Linear stability analysis The stability of the homogeneous deformation may be investigated by seeking an inhomogeneous solution with small perturbations from the homogeneous solution = h + (t) sin(kx); (27a) = h + (t) sin(kx); (27b) = h + (t) sin(kx); (27c) where k is the wave number of the perturbations, and ( ; ; ) denote the amplitudes of the perturbations, assumed to be small compared to ( h ; h ; h ). The shear stress and the dilatational strain are required to be homogeneous and have no perturbations. This method is commonly used when the homogeneous solution is time-independent; however, it has been employed in time-dependent cases by Clifton (1980), Bai (1982), and Fressengeas and Molinari (1987) for thermo-plastic instability analysis. In those cases, it is assumed that the growth rate of the perturbation is much greater than the rate of the homogeneous solution. Substitutions of Eq. (27) into Eqs. (25), (20), and (23), and retaining only the 6rst order terms of ; , and lead to d 9g 2 2 = −k l ; (28a) dt 9 d 9f = ; (28b) dt 9

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1021 0.04 Normalized shear stress, τ/µ 0.03 0.02 0.01 0 0 0.05 0.1 0.15 0.2 (a) Shear strain, γ 0.01 Free volume concentration, ξ 0.009 0.008 0 0.05 0.1 0.15 0.2 (b) Shear strain, γ Fig. 3. Results from the homogeneous solution of the simple shear problem with normalized strain rate r=R = 10−6 : (a) shear stress versus shear strain; (b) free volume concentration versus shear strain. d f( h ; h ) 1 9g =− − − k 2 l2 ; (28c) dt 6h 3 9 where 9g=9 and 9f=9 are evaluated at the homogeneous solution, ( h ; h ). The time t in Eq. (28) has been scaled by 1=R and the rate functions, f and g, have been scaled accordingly by R. From Eq. (28a), the perturbation to the concentration of free volume will amplify if (9g=9 ) ¿ k 2 l2 . From Eq. (28b), the perturbation to the shear strain will amplify

1022 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 as the perturbation to the concentration of free volume ampli6es. From Eq. (28c), the growth of the perturbation to the free volume concentration induces the growth of compressive normal stress, but the amplitude of the stress decreases as the result of relaxation through plastic 5ow. From the above analysis, we see that the stability of the homogeneous solution de- pends on the perturbation to the free volume concentration, which is governed by three processes: di4usion, annihilation, and creation. The di4usion of free volume is slow for small wave number perturbations (i.e., long wavelengths) and fast for large wave number perturbations (i.e., short wavelengths). The annihilation of free volume mostly depends on temperature, slow at low temperature and fast at high temperature. The stress-driven creation of free volume is slow at low stresses and fast at high stresses. The di4usion and annihilation processes cause the perturbation to decay, and the cre- ation process causes the perturbation to amplify. The stability of the homogeneous deformation is determined by the competition of these three processes. As seen in Eq. (26) and Fig. 3, both the shear stress and the free volume concentra- tion in the homogeneous deformation are changing over the time. Once the combination of the shear stress and free volume satis6es the condition, (9g=9 ) ¿ k 2 l2 , the homoge- neous deformation becomes unstable and the perturbations start to grow. Fig. 4 shows the variation of 9g=9 (scaled by R) from the homogeneous solution for the normalized strain rate r=R = 10−6 . The maximum value of (9g=9 ) de6nes a critical wave number satisfying kc2 l2 = max[9g=9 ]. The homogeneous deformation is stable for k ¿ kc and unstable for k ¡ kc . The critical wave number depends on the prescribed strain rate, as shown in Fig. 5. Note that the linear perturbation analysis is only valid for a short time after instability and cannot predict the whole process of inhomogeneous deformation. Eqs. (22) – (25) must be solved numerically for the complete solution of inhomogeneous deformation. 5.3. Inhomogeneous deformation The deformation of the metallic glass layer will be inhomogeneous if the initial free volume is not uniformly distributed. In practice, the non-uniform distribution of free volume may be the result of quenching processes or due to thermal 5uctuation. Assume a 6nite amplitude disturbance in the form of a Gauss function is added to the initial distribution of free volume, i.e., (x − x0 )2 (x; 0) = i + exp − ; (29) (2 where i is a constant, is the amplitude of the disturbance, x0 is the location, and ( is the characteristic half width. It is assumed that (h such that the boundaries of the layer at x = ± h are far away from the disturbance and therefore, have little e4ect on the evolution of the disturbance. In the following numerical simulation, we take i = 0:008; = 0:001; x0 = 0; ( = 100l, and h = 2000l. The stresses and strains are assumed to be zero in the initial con6guration. Eq. (25) is solved by the 6nite element method and a semi-implicit algorithm is used for the time integration. The integrations with respect to x in Eqs. (22) and (24) are

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1023 Fig. 4. Variation of 9g=9 (scaled by R) from the homogeneous solution of the simple shear problem. 1 10 Normalized critical wave number, kc / 0 10 k > kc: stable -1 10 -2 10 -3 k < kc: unstable 10 -4 10 -8 -6 -4 -2 10 10 10 10 Normalized shear strain rate, r/R Fig. 5. Stability analysis of the homogeneous deformation: critical wave number versus shear strain rate. computed by the Gaussian quadrature. Since the boundary of the layer is far away from the disturbance (h(), the free volume is uniformly distributed near the boundaries and 9 =9x = 0 is assumed at the boundaries. At each time step, the shear stress and the free volume concentration at the next time step are computed from Eqs. (22) and (25), respectively, using the values at the current time step; then, the normal strain is

1024 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 0 02 0.02 0.4 0 35 0.35 0.018 Free volume concentration, ξ 0.3 γave = 0.048 Shear strain, γ 0.016 γave = 0.048 0.25 0.014 0.2 γave = 0.046 0.012 0.15 γave = 0.046 g = 0.044 0.1 ave 0.01 γave = 0.044 γave = 0 0.05 0.008 0 -2000 -1500 -1000 -500 0 500 1000 1500 2000 -2000 -1500 -1000 -500 0 500 1000 1500 2000 (a) Normalized distance from center, x/l (b) Normalized distance from center, x/l -3 x 10 4 Normalized normal stress, σ/µ 3 2 1 0 -1 γave = 0.044 -2 γave = 0.046 -3 γave = 0.048 -4 -2000 -1500 -1000 -500 0 500 1000 1500 2000 (c) Normalized distance from center, x/l Fig. 6. Results from the numerical simulation of the inhomogeneous deformation: distributions of (a) free volume concentration, (b) shear strain and (c) normal stress. computed from Eq. (24), after which the normal stress is computed at each integration point from Eq. (23); the shear strains at the integration points are computed from Eq. (20) although it is not necessary for the computations at the next time step. Figs. 6 and 7 show the results of a numerical simulation of the inhomogeneous deformation with the prescribed average shear strain rate r = 10−6 R. Fig. 6a shows the distributions of the free volume at di4erent time steps, where the time is indicated by the average shear strain, ave = rt. Figs. 6b and c show the distributions of the shear strain and the normal constraining stress. Fig. 7 shows the shear stress versus the average shear strain. At the initial stage of the deformation, the stress is low and the change of the free volume is dominated by the di4usion and annihilation processes. At this stage, the amplitude of the initial disturbance to the free volume concentration decays, the deformation is nearly homogeneous and elastic. As the shear stress increases, the creation process of the free volume becomes more signi6cant. The amplitude of the disturbance starts to grow at ave ≈ 0:04, when the creation process starts to dominate the di4usion and annihilation. As shown in Fig. 6a, the free volume concentration at the center of the disturbance grows much faster than it does elsewhere. Meanwhile, the shear strain grows rapidly at the center, but increases

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1025 0.04 0.035 Normalized shear stress, τ/µ 0.03 0.025 0.02 0.015 0.01 0.005 0 0 0.05 0.1 0.15 0.2 Average shear strain, γave = rt Fig. 7. Variation of the shear stress from the numerical simulation of the inhomogeneous deformation with r=R = 10−6 . The dashed line is from the corresponding homogeneous solution. slowly and even decreases at the other location, which develops a localized distribution of the shear deformation, as shown in Fig. 6b. The inhomogeneous growth of the free volume causes inhomogeneous dilatation of the material, which in turn causes the constraining normal stress, as shown in Fig. 6c. The normal stress is relatively small comparing to the shear stress. As the free volume and shear strain start to localize, the shear stress drops abruptly from a maximum stress, as shown in Fig. 7. As the shear stress drops to a lower level, the di4usion and annihilation processes regain the dominance against the creation process and eventually stop the localization process. Similar behaviors have been observed in the uniaxial compression tests, where shear bands formed, propagated, and then stop (Wright et al., 2001). Finally, the deformation approaches the homogeneous steady state and the distribution of free volume becomes uniform. The results of the numerical simulation are sensitive to several parameters. For in- stance, very di4erent behavior can be obtained if a di4erent value of in Eqs. (12) and (14) is used, or if a di4erent value of the initial free volume concentration ( i ) is used. In some cases, the localization of free volume is so severe that the shear stress drops to zero before the localization stops, a di4erent behavior as observed in the uniaxial tensile tests. 6. Concluding remarks A framework for inhomogeneous deformation in metallic glasses has been presented. The free volume concentration is adopted as the order parameter of the amorphous material systems. The speci6c rate functions for the free volume generation and plastic

1026 R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 5ow depend on the underlying microscopic model, but the framework is generally valid for other models. As an example, the simple shear problem is solved. Both homogeneous and inhomo- geneous solutions are obtained and the results are based on the chosen rate functions, obtained from a simple extension of the microscopic model by Spaepen (1977). The numerical simulation shows the development of the inhomogeneous deformation and the strain localization. Acknowledgements The work at Princeton is supported by the National Science Foundation through Grants CMS-9820713 and CMS-9988788 with Drs. Ken Chong and Jorn Larsen-Basse as the program directors. ZS thanks helpful discussions with Professors A.G. Evans, F. Spaepen, R.H. Dauskardt, and D. Srolovitz. The work at Stanford (WDN) was supported by the Air Force OSce of Scienti6c Research under AFOSR Grant No. F49620-98-1-0260. References Argon, A.S., 1979. Plastic deformation in metallic glasses. Acta Metall. 27, 47–58. Bai, Y.L., 1982. Thermo-plastic instability in simple shear. J. Mech. Phys. Solids 30 (4), 195–207. Chen, H.S., Goldstein, M., 1972. Anomalous viscoelastic behavior of metallic glasses of Pd–Si-Based alloys. J. Appl. Phys. 43 (4), 1642. Clifton, R.J., 1980. Material response to ultra-high loading rates. NRC Report No. 356, US National Material Advisory Board. Cohen, M.H., Turnbull, D., 1959. Molecular transport in liquids and glasses. J. Chem. Phys. 31 (5), 1164–1169. Conner, R.D., Rosakis, A.J., Johnson, W.L., Owen, D.M., 1997. Fracture toughness determination for a beryllium-bearing bulk metallic glass. Scr. Mater. 37 (9), 1373–1378. Davis, L.A., Kavesh, S., 1975. J. Mater. Sci. 10, 453. Flores, K.M., Dauskardt, R.H., 1999. Enhanced toughness due to stable crack tip damage zones in bulk metallic glass. Scr. Mater. 41 (9), 937–943. Flores, K.M., Dauskardt, R.H., 2001. Mean stress e4ects on 5ow localization and failure in a bulk metallic glass. Acta Mater. 49 (13), 2527–2537. Fressengeas, C., Molinari, A., 1987. Instability and localization of plastic 5ow in shear at high strain rates. J. Mech. Phys. Solids 35 (2), 185–211. Gilbert, C.J., Ritchie, R.O., Johnson, W.L., 1997. Fracture toughness and fatigue-crack propagation in a Zr–Ti–Ni–Cu–Be bulk metallic glass. Appl. Phys. Lett. 71 (4), 476–478. Hays, C.C., Kim, C.P., Johnson, W.L., 2000. Microstructure controlled shear band pattern formation and enhanced plasticity of bulk metallic glasses containing in situ formed ductile phase dendrite dispersions. Phys. Rev. Lett. 84 (13), 2901–2904. Hufnagel, T.C., El-Deiry, P., Vinci, R.P., 2000. Development of shear band structure during deformation of a Zr 57 Ti5 Cu20 Ni8 Al10 bulk metallic glass. Scr. Mater. 43 (12), 1071–1075. Johnson, W.L., 1999. Bulk glass-forming metallic alloys: science and technology. MRS Bull. 24 (10), 42–56. Klement, W., Willens, R.H., Duwez, P., 1960. Nature 187, 869. Leamy, H.J., Chen, H.S., Wang, T.T., 1972. Plastic 5ow and fracture of metallic glass. Metall. Trans. 3, 699–708. Leng, Y., Courtney, T.H., 1991. Multiple shear band formation in metallic glasses in composites. J. Mater. Sci. 26, 588–592.

R. Huang et al. / J. Mech. Phys. Solids 50 (2002) 1011 – 1027 1027 Lowhaphandu, P., Lewandowski, J.J., 1998. Fracture toughness and notched toughness of bulk amorphous alloy: Zr–Ti–Ni–Cu–Be. Scr. Mater. 38 (12), 1811–1817. Lowhaphandu, P., Montgomery, S.L., Lewandowski, J.J., 1999. E4ects of superimposed hydrostatic pressure on 5ow and fracture of a Zr–Ti–Ni–Cu–Be bulk amorphous alloy. Scr. Mater. 41 (1), 19–24. Maekawa, S., Takashima, K., Shimojo, M., Higo, Y., Swain, M.V., 2000. Fatigue properties for micro-sized Ni–P amorphous alloy specimens. Mat. Res. Soc. Symp. Proc. 605, 247–252. Onugi, M., Inoue, A., Yamaguchi, T., Minamiguchi, H., Iwata, K., 1999. Mater. Jpn. 38, 251. Pampillo, C.A., 1975. Flow and fracture in amorphous alloys. J. Mater. Sci. 10 (7), 1194–1227. Spaepen, F., 1977. A microscopic mechanism for steady state inhomogeneous 5ow in metallic glasses. Acta Metall. 25, 407–415. Steif, P.S., Spaepen, F., Hutchinson, J.W., 1982. Strain localization in amorphous metals. Acta Metall. 30, 447–455. Steif, P.S., 1983. Ductile versus brittle behavior of amorphous metals. J. Mech. Phys. Solids 31 (5), 359–388. Taub, A.I., Spaepen, F., 1980. The kinetics of structural relaxation of a metallic glass. Acta Metall. 28, 1781–1788. Turnbull, D., Cohen, M.H., 1961. Free-volume model of the amorphous phase: glass transition. J. Chem. Phys. 34 (1), 120–125. Turnbull, D., Cohen, M.H., 1970. On the free volume model of the liquid–glass transition. J. Chem. Phys. 52 (6), 3038–3041. Vaks, V.G., 1991. Possible mechanism for formation of localized shear bands in amorphous alloys. Phys. Lett. A 159, 174–178. Wright, W.J., Saha, R., Nix, W.D., 2001. Deformation mechanisms of the Zr 40 Ti14 Ni10 Cu12 Be24 bulk metallic glass. Mater. Trans. JIM 42 (4), 642–649.

You can also read